Zeolites are microporous, aluminosilicate minerals commonly used as commercial adsorbents and catalysts. The term zeolite was originally coined in 1756 by Swedish mineralogist Axel Fredrik Cronstedt, who observed that rapidly heating the material, believed to have been stilbite, produced large amounts of steam from water that had been adsorbed by the material. Based on this, he called the material zeolite, from the Greek (zé?), meaning "to boil" and (líthos), meaning "stone". The classic reference for the field has been Breck's book Zeolite Molecular Sieves: Structure, Chemistry, And Use.
Zeolites occur naturally but are also produced industrially on a large scale. As of December 2018 Every new zeolite structure that is obtained is examined by the International Zeolite Association Structure Commission and receives a three letter designation., 245 unique zeolite frameworks have been identified, and over 40 naturally occurring zeolite frameworks are known.
Zeolites have a porous structure that can accommodate a wide variety of cations, such as Na+, K+, Ca2+, Mg2+ and others. These positive ions are rather loosely held and can readily be exchanged for others in a contact solution. Some of the more common mineral zeolites are analcime, chabazite, clinoptilolite, heulandite, natrolite, phillipsite, and stilbite. An example of the mineral formula of a zeolite is: ·2H2O, the formula for natrolite. These cation exchanged zeolites possess different acidity and catalyse several acid catalysis.
Natural zeolites form where volcanic rocks and ash layers react with alkaline groundwater. Zeolites also crystallize in post-depositional environments over periods ranging from thousands to millions of years in shallow marine basins. Naturally occurring zeolites are rarely pure and are contaminated to varying degrees by other minerals, metals, quartz, or other zeolites. For this reason, naturally occurring zeolites are excluded from many important commercial applications where uniformity and purity are essential.
Zeolites are the aluminosilicate( and ) members of the family of microporous solids known as "molecular sieves", and mainly consist of Si, Al, O, and metals including Ti, Sn, Zn, and so on. The term molecular sieve refers to a particular property of these materials, i.e., the ability to selectively sort molecules based primarily on a size exclusion process. This is due to a very regular pore structure of molecular dimensions. The maximum size of the molecular or ionic species that can enter the pores of a zeolite is controlled by the dimensions of the channels. These are conventionally defined by the ring size of the aperture, where, for example, the term "8-ring" refers to a closed loop that is built from eight tetrahedrally coordinated silicon (or aluminium) atoms and 8 oxygen atoms. These rings are not always perfectly symmetrical due to a variety of causes, including strain induced by the bonding between units that are needed to produce the overall structure, or coordination of some of the oxygen atoms of the rings to cations within the structure. Therefore, the pores in many zeolites are not cylindrical.
Industrially important zeolites are produced synthetically. Typical procedures entail heating aqueous solutions of alumina and silica with sodium hydroxide. Equivalent reagents include sodium aluminate and sodium silicate. Further variations include changes in the cations to include quaternary ammonium cations.
Synthetic zeolites hold some key advantages over their natural analogues. The synthetic materials are manufactured in a uniform, phase-pure state. It is also possible to produce zeolite structures that do not appear in nature. Zeolite A is a well-known example. Since the principal raw materials used to manufacture zeolites are silica and alumina, which are among the most abundant mineral components on earth, the potential to supply zeolites is virtually unlimited.
Conventional open-pit mining techniques are used to mine natural zeolites. The overburden is removed to allow access to the ore. The ore may be blasted or stripped for processing by using tractors equipped with ripper blades and front-end loaders. In processing, the ore is crushed, dried, and milled. The milled ore may be air-classified as to particle size and shipped in bags or bulk. The crushed product may be screened to remove fine material when a granular product is required, and some pelletized products are produced from fine material.
As of 2016tonnes. Major producers in 2010 included China (2 million tonnes), South Korea (210,000 t), Japan (150,000 t), Jordan (140,000 t), Turkey (100,000 t) Slovakia (85,000 t) and the United States (59,000 t). The ready availability of zeolite-rich rock at low cost and the shortage of competing minerals and rocks are probably the most important factors for its large-scale use. According to the United States Geological Survey, it is likely that a significant percentage of the material sold as zeolites in some countries is ground or sawn volcanic tuff that contains only a small amount of zeolites. Some examples of such usage include dimension stone (as an altered volcanic tuff), lightweight aggregate, pozzolanic cement, and soil conditioners.the world's annual production of natural zeolite approximates 3 million
There are over 200 synthetic zeolites that have been synthesized by a process of slow crystallization of a silica-alumina gel in the presence of alkalis and organic templates. Many more such structures could theoretically be made. In addition to variations in structures, zeolites can also be made with a variety of other atoms in them to make them chemically interesting and active. Some examples of the so-called heteroatoms that have been incorporated include germanium, iron, gallium, boron, zinc, tin, and titanium. One of the important processes used to carry out zeolite synthesis is sol-gel processing. The product properties depend on reaction mixture composition, pH of the system, operating temperature, pre-reaction 'seeding' time, reaction time as well as the templates used. In sol-gel process, other elements (metals, metal oxides) can be easily incorporated. The silicalite sol formed by the hydrothermal method is very stable. The ease of scaling up this process makes it a favorite route for zeolite synthesis.
Computer calculations have predicted that millions of hypothetical zeolite structures are possible. However, only 232 of these structures have been discovered and synthesized so far, so many zeolite scientists question why only this small fraction of possibilities are being observed. This problem is often referred to as "the bottleneck problem". Currently there are a number of theories attempting to explain the reasoning behind this question.
Zeolites are widely used as ion-exchange beds in domestic and commercial water purification, softening, and other applications. In chemistry, zeolites are used to separate molecules (only molecules of certain sizes and shapes can pass through), and as traps for molecules so they can be analyzed.
Zeolites are also widely used as catalysts and sorbents. Their well-defined pore structure and adjustable acidity make them highly active in a large variety of reactions.
Zeolites have the potential of providing precise and specific separation of gases, including the removal of H2O, CO2 and SO2 from low-grade natural gas streams. Other separations include noble gases, N2, O2, freon and formaldehyde.
On-board oxygen generating systems (OBOGS) and Oxygen concentrators use zeolites in conjunction with pressure swing adsorption to remove nitrogen from compressed air in order to supply oxygen for aircrews at high altitudes, as well as home and portable oxygen supplies.
Synthetic zeolites, as other mesoporous materials (e.g. MCM-41), are widely used as catalysts in the petrochemical industry, for instance in fluid catalytic cracking and hydrocracking. Zeolites confine molecules in small spaces, which causes changes in their structure and reactivity. The acidic forms of zeolites prepared are often powerful solid-state solid acids, facilitating a host of acid-catalyzed reactions, such as isomerisation, alkylation, and cracking.
Catalytic cracking uses reactor and a regenerator. Feed is injected onto hot, fluidized catalyst where large gasoil molecules are broken into smaller gasoline molecules and olefins. The vapor-phase products are separated from the catalyst and distilled into various products. The catalyst is circulated to a regenerator where air is used to burn coke off the surface of the catalyst that was formed as a byproduct in the cracking process. The hot regenerated catalyst is then circulated back to the reactor to complete its cycle.
Zeolites have uses in advanced nuclear-waste reprocessing methods, where their micro-porous ability to capture some ions while allowing others to pass freely allows many fission products to be efficiently removed from the waste and permanently trapped. Equally important are the mineral properties of zeolites. Their alumino-silicate construction is extremely durable and resistant to radiation even in porous form. Additionally, once they are loaded with trapped fission products, the zeolite-waste combination can be hot pressed into an extremely durable ceramic form, closing the pores and trapping the waste in a solid stone block. This is a waste form factor that greatly reduces its hazard compared to conventional reprocessing systems. Zeolites are also used in the management of leaks of radioactive materials. For example, in the aftermath of the Fukushima Daiichi nuclear disaster, sandbags of zeolite were dropped into the seawater near the power plant to adsorb radioactive caesium which was present in high levels.
The German group Fraunhofer e.V. announced that they had developed a zeolite substance for use in the biogas industry for long-term storage of energy at a density 4x more than water. Ultimately, the goal is to be able to store heat both in industrial installations and in small combined heat and power plants such as those used in larger residential buildings.
Zeolites can be used as solar thermal collectors and for adsorption refrigeration. In these applications, their high heat of adsorption and ability to hydrate and dehydrate while maintaining structural stability is exploited. This hygroscopic property coupled with an inherent exothermic (energy releasing) reaction when transitioning from a dehydrated to a hydrated form make natural zeolites useful in harvesting waste heat and solar heat energy. Zeolites are also used as a molecular sieve in cryosorption style vacuum pumps.
The largest single use for zeolite is the global laundry detergent market. This amounted to 1.44 million metric tons per year of anhydrous zeolite A in 1992.
Synthetic zeolites are used as an additive in the production process of warm mix asphalt concrete. The development of this application started in Germany in the 1990s. They help by decreasing the temperature level during manufacture and laying of asphalt concrete, resulting in lower consumption of fossil fuels, thus releasing less carbon dioxide, aerosols, and vapours. The use of synthetic zeolites in hot mixed asphalt leads to easier compaction and, to a certain degree, allows cold weather paving and longer hauls.
When added to Portland cement as a pozzolan they can reduce chloride permeability and improve workability. They reduce weight and help moderate water content while allowing for slower drying which improves break strength. When added to lime mortars and lime-metakaolin mortars, synthetic zeolite pellets can act simultaneously as pozzolanic material and water reservoir.
Debbie Meyer Green Bags, a produce storage and preservation product, uses a form of zeolite as its active ingredient. The bags are lined with zeolite to adsorb ethylene, which is intended to slow the ripening process and extend the shelf life of produce stored in the bags.
Thomsonites, one of the rarer zeolite minerals, have been collected as gemstones from a series of lava flows along Lake Superior in Minnesota and to a lesser degree in Michigan, U.S. Thomsonite nodules from these areas have eroded from basalt lava flows and are collected on beaches and by scuba divers in Lake Superior.
These thomsonite nodules have concentric rings in combinations of colors: black, white, orange, pink, purple, red, and many shades of green. Some nodules have copper inclusions and rarely will be found with copper "eyes". When polished by a lapidary the thomsonites sometimes display a "cat's eye" effect (chatoyancy).
Research into and development of the many biochemical and biomedical applications of zeolites, particularly the naturally occurring species heulandite, clinoptilolite and chabazite has been ongoing.
Zeolite-based oxygen concentrator systems are widely used to produce medical-grade oxygen. The zeolite is used as a molecular sieve to create purified oxygen from air using its ability to trap impurities, in a process involving the adsorption of nitrogen, leaving highly purified oxygen and up to 5% argon.
In agriculture, clinoptilolite (a naturally occurring zeolite) is used as a soil treatment. It provides a source of slowly released potassium. If previously loaded with ammonium, the zeolite can serve a similar function in the slow release of nitrogen. Zeolites can also act as water moderators, in which they will absorb up to 55% of their weight in water and slowly release it under the plant's demand. This property can prevent root rot and moderate drought cycles. Clinoptilolite has also been added to chicken food: the absorption of water and ammonia by the zeolite made the birds' droppings drier, less odoriferous and hence easier to handle.
Pet stores market zeolites for use as filter additives in aquaria, where they can be used to adsorb ammonia and other nitrogenous compounds. They must be used with some care, especially with delicate tropical corals that are sensitive to water chemistry and temperature. Due to the high affinity of some zeolites for calcium, they may be less effective in hard water and may deplete calcium. Zeolite filtration is also used in some marine aquaria to keep nutrient concentrations low for the benefit of corals adapted to nutrient-depleted waters.
Where and how the zeolite was formed is an important consideration for aquarium applications. Most Northern hemisphere natural zeolites were formed when molten lava came in contact with sea water, thereby "loading" the zeolite with Na (sodium) sacrificial ions. The mechanism is well known to chemists as ion exchange. These sodium ions can be replaced by other ions in solution, thus the takeup of nitrogen in ammonia, with the release of the sodium. A deposit near Bear River in southern Idaho, (US) is a fresh water variety (Na < 0.05%). Southern hemisphere zeolites are typically formed in freshwater and have a high calcium content.